Facile and green reduction of covalently PEGylated nanographene oxide via a ‘water-only’ route for high-efficiency photothermal therapy
© Chen et al.; licensee Springer. 2014
Received: 23 November 2013
Accepted: 10 February 2014
Published: 18 February 2014
A facile and green strategy is reported for the fabrication of nanosized and reduced covalently PEGylated graphene oxide (nrGO-PEG) with great biocompatibility and high near-infrared (NIR) absorbance. Covalently PEGylated nGO (nGO-PEG) was synthesized by the reaction of nGO-COOH and methoxypolyethylene glycol amine (mPEG-NH2). The neutral and purified nGO-PEG solution was then directly bathed in water at 90°C for 24 h without any additive to obtain nrGO-PEG. Covalent PEGylation not only prevented the aggregation of nGO but also dramatically promoted the reduction extent of nGO during this reduction process. The resulting single-layered nrGO-PEG sheets were approximately 50 nm in average lateral dimension and exhibited great biocompatibility and approximately 7.6-fold increment in NIR absorption. Moreover, this facile reduction process repaired the aromatic structure of GO. CCK-8 and flow cytometry (FCM) assays showed that exposure of A549 cells to 100 μg/mL of nrGO-PEG for 2 h, exhibiting 71.5% of uptake ratio, did not induce significant cytotoxicity. However, after irradiation with 808 nm laser (0.6 W/cm2) for 5 min, the cells incubated with 6 μg/mL of nrGO-PEG solution showed approximately 90% decrease of cell viability, demonstrating the high-efficiency photothermal therapy of nrGO-PEG to tumor cells in vitro. This work established nrGO-PEG as a promising photothermal agent due to its small size, great biocompatibility, high photothermal efficiency, and low cost.
KeywordsGraphene oxide Covalent functionalization Green reduction Near-infrared absorbance Bioapplication Photothermal therapy
Graphene oxide (GO), a low-cost carbon nanomaterial synthesized from graphite with fascinating physical and chemical properties, has been widely developed in the past several decades [1–4]. Its unique nanostructure holds great promise for potential applications in biomedicine such as microbial detection, nanocarrier systems, and photosensitizer [5–9]. However, GO is unstable and tends to aggregate in water due to the Van der Waals interaction and strong π-π stacking between GO nanosheets. To render superior stability in aqueous solution, GO is generally ultrasonicated to nanosized GO (nGO) and then functionalized covalently by biocompatible and nontoxic surfactant such as polyethylene glycol (PEG) and p-aminobenzenesulfonic acid via amido bond [10–12]. Covalently PEGylated nGO (nGO-PEG) can be used as nanocarriers for aromatic antitumor drugs such as doxorubicin (DOX), SN38, and camptothecin (CPT) through π-π stacking between drugs and nGO surface [8, 13, 14]. Recently, nGO-PEG has also been used as photoabsorbing agent for photothermal therapy (PTT) [15–17]. However, the very low near-infrared (NIR) absorption of nGO-PEG leads to the inefficient ablation of large tumors or tumors deeply located inside the body and the usage of relatively high NIR laser power for the PTT of nGO-PEG [2, 15–19].
The reduced nGO (nrGO) has attracted great interest especially in PTT [20–24] since the reduction of nGO by removing oxygen-containing groups can result in a dramatic increment in NIR absorption. Toxic chemical reducing reagents, such as sodium borohydride, hydrazine, and its derivatives, are usually used to reduce nGO. Although the nrGO produced by chemical reduction methods have high conductivity and C/O ratio, the intense agglomeration and the residual toxic reduction reagent limit its bioapplication [20, 21, 25, 26]. Recently, some green strategies have been developed to produce soluble nrGO. Natural extracts like green tea, gelatin, and spinach leaf can act as both the green reduction reagents and functionalization reagents [23, 27–29]. Strong alkaline and alcohols were also utilized to reduce nGO [30, 31]. In addition, a ‘water-only’ green reduction route to produce graphene by hydrothermal dehydration under high temperature of 180°C was reported, in which the overheated supercritical (SC) water in sealed container acted as reducing agent .
Herein, we developed a more facile and green strategy to obtain stable nrGO-PEG by reducing nGO-PEG in water. In addition, to the ability to recover π-conjugation via repairing the postreduction defects, our approach has three marked advantages over the previously reported green reduction processes: (1) the reduction process requires very simple setup and low temperature, that is, basically a water bath kettle, (2) the resulting nrGO-PEG exhibits great biocompatibility and noncytotoxicity, making it a promising candidate for biorelated application, (3) the resulting nrGO-PEG has an approximately 7.6-fold increment in NIR absorption, making nrGO-PEG a potential photosensitizer for PTT.
Synthesis of nGO-PEG
The nGO-PEG was synthesized following previous studies in our laboratory [13, 16]. In brief, GO was made by a modified Hummer's method utilizing expandable graphite flake (XF NANO Co., Ltd., Nanjing, China) [33, 34]. nGO solution was prepared by sonication of GO flake. NaOH (1.2 g) and Cl-CH2-COOH (1.0 g) were added to nGO suspension (approximately 2 mg/mL) and sonicated for 30 min to obtain carboxylation nGO (nGO-COOH). The resulting nGO-COOH suspension was neutralized and purified by repeatedly rinsing and filtration. Methoxypolyethylene glycol amine (5 kDa MW, mPEG-NH2, PEG BIO Co., Ltd., Suzhou, Jiangsu, China) and nGO-COOH suspension reacted at pH of 6 and then, 1-ethyl-3-(3-dimethylaminopropyl)carbodiimide (4 mM) and N-hydroxysuccinimide (10 mM) (EDC and NHS, Sigma, St. Louis, MO, USA) were added to the above suspension. The nGO-PEG was purified by centrifuging with 30 kDa ultracentrifuge tube (Millipore, Billerica, MA, USA) and dialyzed against distilled water for overnight to remove any ions, and then, by centrifuging the solution of the mixture at 12,000× g for 30 min to remove any unstable aggregates.
Synthesis of nrGO-PEG
Twenty milliliters of nGO-PEG solution (approximately 0.5 mg/mL) was transferred to a sealed glass bottle and then bathed at different temperature for 24 h or bathed at 90°C for different times. The resulting nrGO-PEG solution was centrifuged at 6,000× g for 30 min to remove any unstable aggregates and stored at 4°C for further use.
The GO, nGO, nGO-PEG, and nrGO-PEG sheets were imaged with atomic force microscopy (AFM, Agilent Technologies 5500, Santa Clara, CA, USA) on a mica substrate. UV-vis spectra were performed by a UV-vis spectrometer (Lambda 35, Perkin-Elmer, Waltham, MA, USA) with a 1-cm quartz cuvette. Fourier transform infrared (FTIR) spectra were recorded on a FTIR spectrometer (Bruker Tensor 27, Karlsruhe, Germany). Raman spectra were taken with a Renishaw (New Mills, UK) inVia micro-Raman spectroscopy system equipped with a 514.5-nm Ar+ laser. The images of all samples were recorded using a digital camera (Nikon, Tokyo, Japan) with 1,280 × 1,280 pixels resolution.
Fluorescence labeling of nrGO-PEG and cell uptake assay
The nrGO-PEG was labeled by fluorescein isothiocyanate (FITC, Sigma). In brief, the solution of nrGO-PEG (approximately 0.5 mg/mL) was mixed with 0.1 mL FITC (13 mM) dissolved in DMSO and then stirred overnight at room temperature. The resulting mixtures labeled with FITC were filtrated through 30 kDa filters to remove excess unbound FITC and centrifuged at 12,000× g for 30 min to eliminate solid aggregated FITC. The obtained nrGO-PEG/FITC was re-dispersed in distilled water. The whole procedures were operated in the dark place.
A549 cells (1 × 105 cells) were incubated with 100 μg/mL of nrGO-PEG/FITC and free FITC for 2 h, respectively, in the dark. After that, the cells were rinsed by phosphate buffered saline (PBS) five times. Fluorescence emission from FITC was observed using a confocal microscope (LSM 510/ConfoCor 2, Zeiss, Jena, Germany). FITC was excited at 488 nm laser with an Ar-Ion laser (reflected by a beam splitter HFT 488 nm), and fluorescence emission was recorded by a 505 to 550-nm IR band-pass filter. The uptake ratio of nrGO-PEG by A549 cells were measured by flow cytometry (FCM, FACSCantoII, Becton Drive, New Jersey, USA) using FITC labeled on nrGO-PEG, and for each FCM analysis, 10,000 events were recorded.
The nrGO-PEG solution was diluted to a desired concentration of 3, 6, 10, 20, and 30 μg/mL with distilled water. The above samples, 3 μg/mL nGO-PEG, and distilled water were continuously irradiated by 808 nm NIR laser with the power density of 0.6 W/cm2 for 8 min. Temperature was measured by a thermocouple thermometer (Fluke 51II, Lake Mary, FL, USA) every other 30 s. In addition, the temperature of water, 3 μg/mL nGO-PEG, and nrGO-PEG solution after the irradiation were also measured by infrared thermal camera (TVS200EX, NEC, Minato, Tokyo, Japan). All the experiments were conducted at room temperature.
Cell culture and cytotoxicity assay
A549 cell line obtained from the Department of Medicine, Jinan University (Guangzhou, China) was cultured in Dulbecco's modified Eagle's medium (DMEM, Gibco, Grand Island, NY, USA) supplemented with 10% fetal calf serum (FCS) in 5% CO2, 95% air at 37°C in a humidified incubator.
For cytotoxicity assay, approximately 5,000 A549 cells/well were plated in 96-well plate with 100 μL medium and cultured for 24 h, and then, various concentrations of nGO-PEG and nrGO-PEG were added to the wells. For photothermal therapy, adherent cells were incubated at various concentrations of nGO-PEG and nrGO-PEG for 2 h and then were irradiated by 808 nm semiconductor laser with the power density of 0.6 W/cm2 for 5 min. The relative cell viability was assessed by Cell Counting Kit-8 (CCK-8, Dojindo, Kamimashiki-gun, Kumamoto, Japan) assay as described previously  and determined by a 96-well plate reader (INFINITE M200, Tecan, Seestrasse, Männedorf, Switzerland) at an absorbance value of 450 nm. All experiments were performed in quadruple occasion.
Cell death assay
A549 cells were cultured in 48-wells plate for 24 h and treated with different concentrations of nGO-PEG and nrGO-PEG for 2 h and then were irradiated by 808 nm semiconductor laser with the power density of 0.6 W/cm2 for 5 min. The living and dead cells in the medium were harvested and washed with PBS and then measured by FCM using AnnexinV-FITC/PI apoptosis detection kit (Bender Medsystems, Vienna, Austria) as previously described , and 10,000 events were recorded for each FCM analysis.
Results and discussion
Synthesis and characterization of nGO-PEG and nrGO-PEG
To make a well-dispersed and stable nGO solution with high NIR absorbance for bioapplication, we have developed a facile and green reduction method to prepare nrGO-PEG.
Step 1: PEGylation of nGO. GO was obtained by oxidization of graphite according to the modified Hummers' method and sonication of GO, resulting in nGO . PEGylation of nGO is usually performed to improve the stability of nGO under physiological conditions [8, 36]. In the present strategy, mPEG-NH2 was introduced to covalently conjugate with nGO-COOH by chemical reaction between -NH2 groups and carboxyl groups under the participation of NHS and EDC, resulting in nGO-PEG .
Step 2: green reduction of nGO-PEG. The stable neutral nGO-PEG solution was bathed in water at 90°C for 24 h.
Next, we reduced nGO-PEG by transferring 20 mL nGO-PEG solution (approximately 0.5 mg/mL) to sealed glass bottles that were then bathed at 4°C, 37°C, 50°C, 70°C, 90°C, and 100°C respectively for 24 h. It was found that the color of nGO-PEG solution at 4°C, 37°C, and 50°C remained nearly unchanged but changed to black brown and dark black at 70°C, 90°C, and 100°C, respectively (Figure 2B inset), indicating the reduction reaction at the temperature range of 70°C to 100°C. The color change from brown to dark black was evident for the reduction of nGO [28, 32]. Consistent to the color change, UV-vis spectra revealed that the nGO-PEG solution bathed at 70°C, 90°C, and 100°C, respectively, for 24 h showed approximately 3.1, approximately 7.6, and approximately 7.8-fold increment in NIR absorption at 808 nm (Figure 2B). Moreover, bathing at 70°C to 100°C for 24 h resulted in a red-shift of the peak at 230 to 261 nm (Figure 2B), indicating partial restoration of the π-conjugation network of carbon structure. In addition, disappearance of the weak shoulder peak at 300 nm (Figure 2B) reflected the effect of deoxygenation [28, 32]. Although the nrGO-PEG suspension obtained at 100°C had an approximately 7.8-fold increment in NIR absorption, it showed some aggregations (Figure 2B inset), likely due to the complete removal of oxygen groups and amido bond of nGO-PEG [31, 32]. Subsequently, we also evaluated the effect of reduction time at 90°C on the reduction extent and found that the color of nGO-PEG solution changed from black brown to dark black with increasing bathing time (Figure 2C inset), and UV-vis spectra showed that the nGO-PEG solution bathed for 24 h had higher NIR absorption than others (Figure 2C).
As control, we next assessed the effect of this reduction method on both nGO and nGO-COOH solutions. In brief, nGO and nGO-COOH solutions were bathed at 90°C for 24 h. UV-vis spectra showed that nGO and nGO-COOH had approximately 3.1 and approximately 3.4-fold increment in NIR absorbance (at 808 nm) (Figure 2D), which was further verified by the color change (darkening) of nGO and nGO-COOH solutions (Figure 2D inset). After reduction, the absorption peak (230 nm) of nGO and nGO-COOH red-shifted to approximately 238 nm and the shoulder peak (300 nm) nearly disappeared (Figure 2D). As shown in Figure 2A,D, carboxylation of nGO and carboxyl group did not affect the reduction extent of nGO. Although nGO and nGO-COOH could be reduced by this green reduction method (Figure 2D), the reduced nGO and nGO-COOH showed intense aggregations and relative low NIR absorbance (Figure 2B,C,D inset), indicating that the endogenous PEG chains of nGO-PEG remarkably strengthened the reduction extent of nGO during this facile and green reduction process.
Raman spectroscopy was used to characterize nGO, nGO-COOH, nGO-PEG, and nrGO-PEG (Figure 3B). The typical features in Raman spectra are the G band at 1,600 cm−1 and the D band at 1,350 cm−1. The G band is usually assigned to the E2g phonon of C sp2 atoms , while the prominent D band is an indication of disorder corresponding to defects associated with vacancies, grain boundaries, and amorphous carbon species [42, 43]. As shown in Figure 3B, the intensity ratio (ID/IG) of D band to G band of nGO, nGO-COOH, nGO-PEG, and nrGO-PEG were about 0.948, 0.953, 0.951, and 0.832, respectively. Obviously, nGO-COOH and nGO-PEG had similar ID/IG value with that of nGO, indicating that both carboxylation and PEGylation did not destroy the aromatic structures of nGO. However, the ID/IG value of nrGO-PEG was much lower than that of nGO, suggesting that the reduction reaction in this facile and green reduction strategy developed here was also able to recover the aromatic structures by repairing defects. It is reported that the ID/IG ratio of chemically reduced nGO is higher than that of as-made GO due to the presence of unrepaired defects after the removal of oxygen moieties [25, 31, 44]. Therefore, the green reduction approach reported here was more effective in repairing the sp2 network. Taking into account the relationship of ID/IG with the extent of π-conjugation and the concentration of defects on GO, the nrGO-PEG obtained by this green reduction method showed more integrated π-conjugation network, which is favorable for loading much more aromatic molecules via π-π stacking.
Photothermal effect and biocompatibility
Recently, Robinson and coworkers reported a chemical reduction method for nGO-PEG by using hydrazine monohydrate as reduction reagent . The nrGO-PEG obtained by this chemical reduction method afforded approximately 6.5-fold increase in NIR absorbance and 26°C increase under 5 min of 808 nm laser irradiation (0.6 W/cm2), but it aggregated in the solution due to the removal of functional groups from GO sheet . Therefore, the nrGO-PEG obtained by this chemical reduction approach must be resuspended by functionalized PEG to increase its biocompatibility for bioapplication [20, 21]. In contrast, the nrGO-PEG obtained by the present green reduction approach had not only approximately 7.6-fold increment in NIR absorbance and 43°C increase under the same laser irradiation (at 808 nm) (Figure 2B,C) but also very great biocompatibility (Figure 2B, C and 5).
Moreover, some natural extracts and nontoxic reagents including gelatin, NaOH, or KOH and alcohols have been also used to reduce GO [28, 30, 31]. Although these green reduction methods need low temperature (about 50°C to 100°C) and short react time (below 24 h), the obtained rGO showed relative bad stability in water (keep stable for less than 1 month). In contrast, the nrGO-PEG prepared with our green method could keep stable for at least 3 months (Figure 5), which is in favor of long-term bioapplication.
Cellular uptake and in vitro photothermal therapy
To determine the cytotoxicity of nGO-PEG and nrGO-PEG under laser irradiation, A549 cells were incubated with various concentrations of nGO-PEG and nrGO-PEG solution for 2 hand then irradiated by 808 nm laser (0.6 W/cm2) for 5 min. CCK-8 assay showed that the laser irradiation did not induce significant cytotoxicity for control cells but induced approximately 35% decrease of cell viability for the cells incubated with 3 μg/mL of nrGO-PEG and approximately 90% decrease of cell viability for the cells incubated with 6 μg/mL nrGO-PEG (Figure 7B), further demonstrating the great PTT effect of nrGO-PEG. As control, the PTT effect of 3 and 6 μg/mL of nGO-PEG were remarkably lower than that of nrGO-PEG (Figure 7B). Moreover, FCM analysis with FITC Annexin V and propidium iodide staining was also used to examine the cell death induced by the photothermal effect of nGO-PEG and nrGO-PEG. As seen in Figure 7C, Q1 + Q2, Q3, and Q4 represented the regions of dead cells, living cells, and early apoptotic cells, respectively [8, 47]. Consistent to the cytotoxicity assay (Figure 7B), laser irradiation did not induce significant cell death for control cells but induced remarkable cell death for the cells cultured with nGO-PEG or nrGO-PEG (6 μg/mL) for 2 h (Figure 7C). Moreover, after the laser irradiation, the cells cultured with nrGO-PEG presented much more dead cells compared with the cells cultured with nGO-PEG (Figure 7C). These in vitro results further demonstrate that the nrGO-PEG obtained by the present green reduction approach may be a great photosensitizer for PTT.
In this work, we have developed a facile and green approach toward biocompatible and controlled reduction of nGO-PEG to nrGO-PEG solution. Covalent PEGylation not only prevents the aggregation of nGO but also dramatically promotes the reduction extent of nGO. This water-only reduction route is very convenient, nontoxic, and environment-friendly and has the ability to recover π-conjugation via repairing the postreduction defects. Moreover, the nrGO-PEG with approximately 50 nm in average size obtained by this green reduction approach has approximately 7.6-fold increment in NIR absorbance, great biocompatibility, and high cellular uptake ratio, making it a promising photoabsorbing agent for PTT comparable to carbon nanotubes and gold-based nanomaterials.
Jingqin Chen and Xiaoping Wang are co-authors.
atomic force microscopy
Fouriertransform infrared spectroscopy
methoxypolyethylene glycol amine
reduced graphene oxide.
This work was supported by the National Natural Science Foundation of China (61178078) and Key Project of the Department of Education and Finance of Guangdong Province (cxzd115).
- Dreyer DR, Park S, Bielawski CW, Ruo RS: The chemistry of graphene oxide. Chem Soc Rev 2010, 39: 228–240. 10.1039/b917103gView Article
- Feng L, Liu Z: Graphene in biomedicine: opportunities and challenges. Nanomedicine 2011, 6: 317–324. 10.2217/nnm.10.158View Article
- Zhi X, Fang H, Bao C, Shen G, Zhang J, Wang K, Guo S, Wan T, Cui D: The immunotoxicity of graphene oxides and the effect of PVP-coating. Biomaterials 2013, 34: 5254–5261. 10.1016/j.biomaterials.2013.03.024View Article
- Yang DP, Wang X, Guo X, Zhi X, Wang K, Li C, Huang G, Shen G, Mei Y, Cui D: UV/O3generated graphene nanomesh: formation mechanism, properties and FET studies. J Phys Chem C 2014, 118: 725–731. 10.1021/jp409898dView Article
- Wu C, Zhang Y, Wu X, Yang Y, Zhou X, Wu H: Biological applications of graphene and graphene oxide. Nano Biomed Eng 2012, 4: 157–162.View Article
- Li C, Wang X, Chen F, Zhang C, Zhi X, Wang K, Cui D: The antifungal activity of graphene oxide–silver nanocomposites. Biomaterials 2013, 34: 882–3890.
- Mohanty N, Berry V: Graphene-based single-bacterium resolution biodevice and DNA transistor: interfacing graphene derivatives with nanoscale and microscale biocomponents. Nano Lett 2008, 8: 4469–4476. 10.1021/nl802412nView Article
- Liu Z, Robinson JT, Sun X, Dai H: PEGylated nanographene oxide for delivery of water-insoluble cancer drugs. J Am Chem Soc 2008, 130: 10876–10877. 10.1021/ja803688xView Article
- Tian B, Wang C, Zhang S, Feng L, Liu Z: Photothermally enhanced photodynamic therapy delivered by nano-graphene oxide. ACS Nano 2011, 5: 7000–7009. 10.1021/nn201560bView Article
- Li D, Müller MB, Gilje S, Kaner RB, Wallace GG: Processable aqueous dispersions of graphene nanosheets. Nat Nanotechnol 2008, 3: 101–105. 10.1038/nnano.2007.451View Article
- Wang K, Ruan J, Song H, Zhang J, Wo Y, Guo S, Cui D: Biocompatibility of graphene oxide. Nanoscale Res Lett 2011, 6: 1–8.
- Zhang L, Xia J, Zhao Q, Liu L, Zhang Z: Functional graphene oxide as a nanocarrier for controlled loading and targeted delivery of mixed anticancer drugs. Small 2010, 6: 537–544. 10.1002/smll.200901680View Article
- Zhang W, Guo Z, Huang D, Liu Z, Guo X: Synergistic effect of chemo-photothermal therapy using PEGylated graphene oxide. Biomaterials 2011, 32: 8555–8561. 10.1016/j.biomaterials.2011.07.071View Article
- Yang K, Zhang S, Zhang G, Sun X, Lee ST, Liu Z: Graphene in mice: ultrahigh in vivo tumor uptake and efficient photothermal therapy. Nano Lett 2010, 10: 3318–3323. 10.1021/nl100996uView Article
- O’Neal DP, Hirschb LR, Halas NJ, Paynea JD, West JL: Photo-thermal tumor ablation in mice using near infrared-absorbing nanoparticles. Cancer Lett 2004, 209: 171–176. 10.1016/j.canlet.2004.02.004View Article
- Zhou F, Wu S, Song S, Chen WR, Resasco DE, Xing D: Antitumor immunologically modified carbon nanotubes for photothermal therapy. Biomaterials 2012, 33: 3235–3242. 10.1016/j.biomaterials.2011.12.029View Article
- Zheng X, Zhou F, Wu B, Chen WR, Xing D: Enhanced tumor treatment using biofunctional indocyanine green-containing nanostructure by intratumoral or intravenous injection. Mol Pharm 2012, 9: 514–522. 10.1021/mp200526mView Article
- Dickersona EB, Dreadenb EC, Huang X, El-Sayed IH, Chu H, Pushpanketh S, McDonald JF, El-Sayed MA: Gold nanorod assisted near-infrared plasmonic photothermal therapy (PPTT) of squamous cell carcinoma in mice. Cancer Lett 2008, 269: 57–66. 10.1016/j.canlet.2008.04.026View Article
- Kam NWS, O’Connell M, Wisdom JA, Dai H: Carbon nanotubes as multifunctional biological transporters and near-infrared agents for selective cancer cell destruction. Proc Natl Acad Sci USA 2005, 102: 11600–11605. 10.1073/pnas.0502680102View Article
- Robinson JT, Tabakman SM, Liang Y, Wang H, Casalongue HS, Vinh D, Dai H: Ultrasmall reduced graphene oxide with high near-infrared absorbance for photothermal therapy. J Am Chem Soc 2011, 133: 6825–6831. 10.1021/ja2010175View Article
- Yang K, Wan J, Zhang S, Tian B, Zhang Y, Liu Z: The influence of surface chemistry and size of nanoscale graphene oxide on photothermal therapy of cancer using ultra-low laser power. Biomaterials 2012, 33: 2206–2214. 10.1016/j.biomaterials.2011.11.064View Article
- Rutter GM, Crain JN, Guisinger NP, Li T, First PN, Stroscio JA: Scattering and interference in epitaxial graphene. Science 2007, 317: 219–222. 10.1126/science.1142882View Article
- Pei S, Cheng HM: The reduction of graphene oxide. Carbon 2012, 50: 3210–3228. 10.1016/j.carbon.2011.11.010View Article
- Hou C, Quan H, Duan Y, Zhang Q, Wang H, Li Y: Facile synthesis of water-dispersible Cu2O nanocrystal–reduced graphene oxide hybrid as a promising cancer therapeutic agent. Nanoscale 2013, 5: 1227–1232. 10.1039/c2nr32938gView Article
- Shin HJ, Kim KK, Benayad A, Yoon SM, Park HK, Jung IS, Jin MH, Jeong HK, Kim JM, Choi JY, Lee YH: Efficient reduction of graphite oxide by sodium borohydride and its effect on electrical conductance. Adv Funct Mater 2009, 19: 1987–1992. 10.1002/adfm.200900167View Article
- Wang Z, Wu S, Zhang J, Chen P, Yang G, Zhou X, Zhang Q, Yan Q, Zhang H: Comparative studies on single-layer reduced graphene oxide films obtained by electrochemical reduction and hydrazine vapor reduction. Nanoscale Res Lett 2012, 7: 1–7. 10.1186/1556-276X-7-1View Article
- Wang Y, Shi Z, Yin J: Facile synthesis of soluble graphene via a green reduction of graphene oxide in tea solution and its biocomposites. ACS Appl Mater Interfaces 2011, 3: 1127–1133. 10.1021/am1012613View Article
- Liu K, Zhang J, Cheng F, Zheng T, Wang C, Zhu J: Green and facile synthesis of highly biocompatible graphene nanosheets and its application for cellular imaging and drug delivery. J Mater Chem 2011, 21: 12034–12040. 10.1039/c1jm10749fView Article
- Gurunathan S, Han JW, Eppakayala V, Dayem AA, Kwon DN, Kim JH: Biocompatibility effects of biologically synthesized graphene in primary mouse embryonic fibroblast cells. Nanoscale Res Lett 2013, 8: 1–13. 10.1186/1556-276X-8-1View Article
- Fan X, Peng W, Li Y, Li X, Wang S, Zhang G, Zhang F: Deoxygenation of exfoliated graphite oxide under alkaline conditions: a green route to graphene preparation. Adv Mater 2008, 20: 4490–4493. 10.1002/adma.200801306View Article
- Dreyer DR, Murali S, Zhu Y, Ruoff RS, Bielawski CW: Reduction of graphite oxide using alcohols. J Mater Chem 2011, 21: 3443–3447. 10.1039/c0jm02704aView Article
- Zhou Y, Bao Q, Tang LAL, Zhong Y, Loh KP: Hydrothermal dehydration for the “green” reduction of exfoliated graphene oxide to graphene and demonstration of tunable optical limiting properties. Chem Mater 2009, 21: 2950–2956. 10.1021/cm9006603View Article
- Hummers WS, Offeman RE Jr: Preparation of graphitic oxide. J Am Chem Soc 1958, 80: 1339–1339. 10.1021/ja01539a017View Article
- Dikin DA, Stankovich S, Zimney EJ, Piner RD, Dommett GHB, Evmenenko G, Nguyen ST, Ruoff RS: Preparation and characterization of graphene oxide paper. Nature 2007, 448: 457–460. 10.1038/nature06016View Article
- Gao W, Xiao F, Wang X, Chen T: Artemisinin induces A549 cell apoptosis dominantly via a reactive oxygen species-mediated amplification activation loop among caspase-9, -8 and −3. Apoptosis 2013, 18: 1201–1213. 10.1007/s10495-013-0857-zView Article
- Sun X, Liu Z, Welsher K, Robinson JT, Goodwin A, Zaric S, Dai H: Nano-graphene oxide for cellular imaging and drug delivery. Nano Res 2008, 1: 203–212. 10.1007/s12274-008-8021-8View Article
- Hermanson GT: Zero-length crosslinkers. In Bioconjugate Techniques. San Diego: Academic; 1996:216–223.
- Stankovich S, Dikin DA, Dommett GHB, Kohlhaas KM, Zimney EJ, Stach EA, Piner RD, Nguyen ST, Ruoff RS: Graphene-based composite materials. Nature 2006, 442: 282–286. 10.1038/nature04969View Article
- Liu X, Tao H, Yang K, Zhang S, Lee ST, Liu Z: Optimization of surface chemistry on single-walled carbon nanotubes for in vivo photothermal ablation of tumors. Biomaterials 2011, 32: 144–151. 10.1016/j.biomaterials.2010.08.096View Article
- Kam NWS, Liu Z, Dai H: Functionalization of carbon nanotubes via cleavable disulfide bonds for efficient intracellular delivery of siRNA and potent gene silencing. J Am Chem Soc 2005, 127: 12492–12493. 10.1021/ja053962kView Article
- Wei DC, Liu YQ, Wang Y, Zhang HL, Huang LP, Yu G: Synthesis of N-doped graphene by chemical vapor deposition and its electrical properties. Nano Lett 2009, 9: 1752–1758. 10.1021/nl803279tView Article
- Ferrari AC, Meyer JC, Scardaci V, Casiraghi C, Lazzeri M, Mauri F, Piscanec S, Jiang D, Novoselov KS, Roth S, Geim AK: Raman spectrum of graphene and graphene layers. Phys Rev Lett 2006, 97: 187401–187405.View Article
- Schönfelder R, Rümmeli MH, Gruner W, Löffler M, Acker J, Hoffmann V, Gemming T, Büchner B, Pichler T: Purification-induced sidewall functionalization of magnetically pure single-walled carbon nanotubes. Nanotechnology 2007, 18: 375601–375609. 10.1088/0957-4484/18/37/375601View Article
- Shen Y, Jing T, Ren W, Zhang J, Jiang Z, Yu Z, Dasari A: Chemical and thermal reduction of graphene oxide and its electrically conductive polylactic acid nanocomposites. Compos Sci Technol 2012, 72: 1430–1435. 10.1016/j.compscitech.2012.05.018View Article
- Abdelsayed V, Moussa S, Hassan HM, Aluri HS, Collinson MM, Samy El-Shall M: Photothermal deoxygenation of graphite oxide with laser excitation in solution and graphene-aided increase in water temperature. J Phys Chem C Lett 2010, 1: 2804–2809. 10.1021/jz1011143View Article
- Yang Q, Pan X, Huang F, Li K: Fabrication of high-concentration and stable aqueous suspensions of graphene nanosheets by noncovalent functionalization with lignin and cellulose derivatives. J Phys Chem C 2010, 114: 3811–3816.View Article
- Vermes I, Haanen C, Steffens-Nakken H, Reutelingsperger C: A novel assay for apoptosis flow cytometric detection of phosphatidylserine expression on early apoptotic cells using fluorescein labelled annexin V. J Immunol Methods 1995, 184: 39–51. 10.1016/0022-1759(95)00072-IView Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.